(2) Ab initio supercell calculations on nitrogen-vacancy center in diamond: its electronic structure and hyperfine tensors Adam Gali,1, 2 Maria Fyta,2 and Efthimios Kaxiras2. arXiv:0803.1267v1 [cond-mat.other] 8 Mar 2008. 1. Department of Atomic Physics, Budapest University of Technology and Economics, Budafoki u ´t 8., H-1111, Budapest, Hungary 2. Department of Physics and School of Engineering and Applied Sciences, Harvard University, Cambridge, Massachusetts 02138, USA. Abstract The nitrogen-vacancy center in diamond is a promising candidate for realizing the spin qubits concept in quantum information. Even though this defect is known for a long time, its electronic structure and other properties have not yet been explored in detail. We study the properties of the nitrogen-vacancy center in diamond through density functional theory within the local spin density approximation, using supercell calculations. While this theory is strictly applicable for ground state properties, we are able to give an estimate for the energy sequence of the excited states of this defect. We also calculate the hyperﬁne tensors in the ground state. The results clearly show that: (i) the spin density and the appropriate hyperﬁne constants are spread along a plane and unevenly distributed around the core of the defect; (ii) the measurable hyperﬁne constants can be found within about 7 ˚ A from the vacancy site. These results have important implications on the decoherence of the electron spin which is crucial in realizing the spin qubits in diamond. PACS numbers: 71.15.Mb, 71.55.Ht, 61.72.Bb, 61.72.Ji. 1.

(3) I.. INTRODUCTION. The nitrogen-vacancy (NV) center in diamond has attracted much attention in recent years, because it has been shown to give rise to a single optically active level within the diamond band gap1,2 , and as such provides an interesting candidate for a qubit for quantum computing applications.3,4,5,6,7,8 Besides providing a single photon source for quantum cryptography,9,10 the NV center is also a promising candidate as an optically coupled quantum register for scalable quantum information processing, such as quantum communication11 and distributed quantum computation.12 In addition, it has been recently demonstrated that proximal nuclear spins can be coherently controlled via hyperﬁne interaction13 and used as a basis for quantum memory with an extremely long coherence time.14 Therefore, knowing the electron-nucleus hyperﬁne interaction and its position-dependence is essential to analyze and optimize coherent control of proximal nuclear spins.15 Experimentally, the hyperﬁne constants of the closest atoms near the vacancy are known from electron paramagnetic resonance (EPR) and electron-nuclear double resonance (ENDOR) studies.16,17 The hyperﬁne interaction between. 13. C isotopes farther from the vacancy. contributes to the coherent electron-nuclear spin states in the measurements.13,14 Ab initio supercell calculations can be a very useful tool for determining the hyperﬁne tensors of a defect. For instance, such calculations have been used to identify the basic vacancy defects in silicon carbide by comparing the measured and calculated hyperﬁne constants.18,19,20,21 In the present paper we focus on the calculation of the full hyperﬁne tensor of the NV center in diamond which is of very high importance for qubit applications. Previous theoretical work has reported a calculation of the hyperﬁne constants of the NV center in a small 64atom supercell,22 but that work determined only the Fermi-contact term rather than the full hyperﬁne tensor. We will show in the Results and Discussion section that the conclusions based on that earlier analysis were adversely aﬀected by the small unit cell size. The larger supercell of 512 atoms employed here does not suﬀer from this limitation and provides a realistic picture for the defect properties, which are in excellent agreement with experimental measurements. The rest of this paper is organized as follows: Section II gives a general discussion of the electronic states of the NV center based on a single-particle picture and the many-body states that can be constructed from this basis. Section III describes the method of the 2.

(4) ﬁrst-principles calculations we performed. Section IV presents and discusses our results concerning the atomic and electronic structure of the defect, as obtained from the ab initio calculations. In Section V we present a detailed discussion of the calculated hyperﬁne interactions. Finally, we give our conclusions on the nature of this defect in Section VI.. II.. THE ELECTRONIC STATES OF THE NV CENTER IN DIAMOND. The electronic structure of NV center in diamond has been discussed in detail in a recent paper23 ; we brieﬂy review the main points here. The NV center was found many years ago in diamond.24 The concentration of NV centers can be enhanced in N-contaminated diamond by irradiation and annealing.24,25 The model of the NV center consists of a substitutional nitrogen atom adjacent to a vacancy in diamond.16,24,25,26 The NV center has a strong optical transition with a zero phonon line (ZPL) at 1.945 eV (637 nm) accompanied by a vibronic band at higher energy in absorption and lower energy in emission. Detailed analysis of the ZPL revealed that the center has trigonal, C3v symmetry.25 Later, an optically induced EPR center was found in diamond which correlated with the NV center.16 The EPR center showed trigonal symmetry with a spin polarized triplet state (S=1). Since the nitrogen atom has ﬁve valence electrons and the S=1 state implies even number of electrons, the NV defect must be charged in the EPR measurement. It was assumed that the NV defect is negatively charged and the extra electron may be donated from isolated substitional nitrogen defects.16 In a recent measurement, the coupling between the NV center and the nitrogen substitional has been indeed detected.27 Loubser and van Wyk16 measured the NV EPR signal just under the optical excitation, based on which they proposed that the spin polarization arises from a singlet electronic system with inter-system crossing to a spin level of a metastable triplet. Redman and co-workers28 detected the NV center in the dark even at 100 K by EPR, from which they concluded that the S=1 state is the ground state of the NV center. Hole burning,29 optically detected magnetic resonance30 and Raman heterodyne measurements31 also showed the S=1 state to be the ground state of the NV center. A group theory analysis based on a single-particle picture can be very useful in understanding the nature of the defect states and the possible optical transitions between them. While the number of electrons in the NV center has been disputed in the literature32,33 a previous ab initio calculation clearly supported the negatively charged NV defect34 as 3.

(5) was originally proposed by Loubser and van Wyk.16 We will also show in the Results and Discussion section that the NV center should be negatively charged. In the NV defect, three carbon atoms have sp3 dangling bonds near the vacancy and three back bonds each to the lattice, while the nitrogen atom has also three back bonds and one dangling bond pointing to the vacant site. Since nitrogen has ﬁve valence electrons the negatively charged NV defect has altogether six electrons around the vacant site. The structure of the NV defect, including the deﬁnition of the symmetry <111> axis, is depicted in Fig. 1. <111>. σ1. (111). σ2. σ3. σ4. FIG. 1: (Color online) The NV center viewed in perspective (left) and along the <111> direction (right); this direction is the C3 symmetry axis of the C3v symmetry group of the defect. The vacant site is indicated by a small pink circle and the neighboring C and N atoms by grey and cyan balls, respectively. The ﬁrst neighbor atoms around the vacant site have sp3 dangling bonds pointing toward the vacant site, which are labeled σi (i = 1, 4), as in the scheme used in the group theory analysis.. The group theory analysis of the six electron model has been worked out previously for this defect.35 We summarize the results using our notation and conventions: Since it is known that the carbon and nitrogen atoms relax outward from the vacancy,22,34 we assume that the overlap between the dangling bonds (σ1−4 ) is negligible, that is, σi σj = δij . σ1−4 are transformed under the operation of C3v point group forming the following orthonormal. 4.

(6) Conduction. ex ex. ey. ey 3.2 eV. a1(2). 2.2 eV a1(2) 0.9 eV VBM 1.2 eV. 1.4 eV VBM 1.2 eV. a1(1) Valence. FIG. 2: (Color online) The calculated spin-resolved single-electron levels with respect to the valence band maximum (VBM) in the ground state of the NV defect. Valence and conduction bands of the host crystal are shown as blue and pink shaded regions, respectively. The levels are labeled as in Eq. (1) and their occupation is given for a negatively charged defect (a total of 6 electrons).. states: √. α 1 − α2 σ4 − √ (σ1 + σ2 + σ3 ) 3 r 1 − α2 (σ1 + σ2 + σ3 ) a1 (2) : φ2 = α σ4 + 3 1 ex : φ3 = √ (2σ1 − σ2 − σ3 ) 6 1 ey : φ4 = √ (σ2 − σ3 ) 2 a1 (1) : φ1 =. (1). where 0 ≤ α ≤ 1is a parameter that determines the extent to which the nitrogen dangling bond is mixed in the φ1 and φ2 defect states. There are two fully symmetric one-electron states (a1 ) and one doubly degenerate e state, with a total occupation of 6 electrons. We note here that the dangling bond of nitrogen is not mixed in the e state but only in the a1 states. It was found by Goss et al.34 using ab initio molecular cluster calculations that the two a1 states are lower in energy than the e state. As a consequence, four electrons occupy the a1 states and two electrons remain for the e state. Our calculated one-electron levels obtained by ab initio supercell calculations are shown in Fig. 2. As can be seen from this 5.

(7) analysis, the natural choice is to put the two remaining electrons in the e level forming an S=1 state (by analogy to Hund’s rule for the p-orbitals of the isolated group IV elements in the Periodic Table). In the C3v point group the total wavefunction has 3 A2 symmetry with S=1. In our special case we choose MS = 1, so both electrons are spin-up electrons in the e level. The C3v symmetry can also be maintained by other occupations of the states. Putting two electrons into four possible quantum states of the degenerate e level, we end up with six possible multiplets (including the degeneracy):. 3. A2 , 1 A1 , and 1 E. By taking the 3 A2. to be the ground state of the defect (as experiments indicate) there is no allowed optical transition to ﬁrst order, since the spin state cannot be changed in a PL process. The φ1 level is relatively deep in the valence band, so to a good approximation we can assume that it does not contribute to the excitation process. However, the φ2 level in the gap is not very far from the e level. If one electron is excited from φ2 into the e level (φ3 or φ4 ) then either a 3 E or a 1 E multiplet is obtained. If both electrons are excited from φ2 to φ3 and φ4 then a fully symmetric 1 A1 state is obtained. The only allowed transition is 3 A2 →3 E to ﬁrst order. The electronic conﬁgurations of these states are explained in Table I. Most of these states were discussed in Ref.35. The MS = ±1 triplet states can be described by a single Slater-determinant. However,. the singlet states (except for the last 1 A1 state) can be described by a linear combination of two Slater-determinants. The two singlet single-Slater-determinant states of the a21 (2)e2 conﬁguration are: 1 (2a) |σ2 σ¯2 σ3 σ¯4 i = √ [1 E(0, y) +3 A2 (0)] 2 1 |σ2 σ¯2 σ3 σ¯3 i = √ [1 E(0, x) +1 A1 (0)] (2b) 2 where 1 E(0, λ) is the multideterminant wavefunction of the singlet E state of MS =0 at λ-row (λ = x or y) in Table I. The singlet single-Slater-determinant state of the a11 (2)e3 conﬁguration is: 1 (3) |σ¯2 σ3 σ4 σ¯4 i = √ [3 E(0, x) +1 E(0, x)] 2 In summary, the following many-body states must be considered: 3 A2 , 1 A1 , 1 E, 3 E, 1 E, and 1 A1 . The two triplet states are orthogonal to each other while the two 1 A1 and the two 1. E states theoretically can be mixed with each other. This will be discussed below. Our. computational method described in the next section cannot take the spin-orbit and spin-spin 6.

(8) TABLE I: The electronic conﬁgurations and the possible total wave functions with C3v symmetry. For simplicity we abbreviate σ2 → 2, etc. in the last column. Overbar in a wavefunction means spin-down electrons, the rest are spin-up electrons. We assume that a1 (1) : σ1 is fully occupied, so we do not show that part of the wave function here. In the second and third columns we give the symmetry of the total wavefunction (Γ) and its spin projection (MS ), respectively. In the case of doubly degenerate representations (E states) we designate which transforms as x or y in the last column. Conﬁguration. Γ. MS. a21 (2)e2. 3A 2. 1. (x,y). |2¯234i √1 [|2¯ 23¯4i + 2. 0. a11 (2)e3. 0. 1E. 0. 3E. 1. 0. -1. 1E. a01 (2)e4. 1A 1. |2¯ 2¯ 34i]. |2¯2¯3¯4i. -1 1A 1. Wave function. 0. √1 [|2¯ 23¯3i + 2. |2¯ 24¯ 4i]. x. √1 [|2¯ 23¯3i − 2. |2¯ 24¯ 4i]. y. √1 [|2¯ 23¯4i − 2. |2¯ 2¯ 34i]. x. |234¯4i. y. |23¯34i. x. √1 [|¯ 234¯4i + 2. y. √1 [|¯ 23¯34i 2. |2¯ 34¯ 4i]. + |23¯ 3¯ 4i]. x. |¯2¯34¯4i. y. |¯23¯3¯4i. x. √1 [|¯ 234¯4i − 2. y. √1 [|¯ 23¯34i 2. |2¯ 34¯ 4i]. − |23¯ 3¯ 4i]. |3¯34¯4i. 0. interaction into account. From the energetic point of view those eﬀects are marginal (within few meV) but they could have important consequences on the possible optical transitions and the spin state of the NV center.23. 7.

(9) III.. COMPUTATIONAL METHOD. We use density functional theory with the local spin density approximation (DFT-LSDA) of Ceperley-Alder36 as parameterized by Perdew and Zunger.37 We employed three diﬀerent codes and somewhat diﬀerent methodologies to carry out the calculations. The geometry of the defect was optimized with the VASP code38,39 and the SIESTA code.40 The latter utilizes numerical atomic orbitals with Troullier-Martins pseudopotentials.41 We applied the high level double-ζ plus polarization functions for both carbon and nitrogen atoms. In the SIESTA calculations no symmetry restriction was applied. The linear combination of atomic orbitals (LCAO) analysis of the defect states is straightforward in this methodology through the wavefunction coeﬃcients obtained directly from the SIESTA calculations. In the VASP calculations we use a plane wave basis set with cutoﬀ 420 eV(≈30 Ry) which is adequate for well converged calculations using projected augmented wave (PAW) pseudopotentials for the C and N atoms.42,43 In the VASP calculations we applied the C3v symmetry, and the energy of the ground state as well as that of the excited states are calculated by setting the appropriate occupation of the defect states in the gap. In the geometry optimization calculations, all the atoms were allowed to relax until the magnitude of the calculated forces was smaller than 0.01 eV/˚ A. The hyperﬁne tensor of the NV center was calculated by the CPPAW code.44 In the CPPAW calculations we used a 30 Ry cutoﬀ for the plane wave basis with PAW projectors which is virtually equivalent with the methodology used in the VASP calculations. Convergence of calculated defect properties with supercell size is an important consideration. For this reason, we have chosen to model the NV center by using a large 512-atom simple cubic supercell. The lattice constant of the supercell (≈14.2 ˚ A) is four times larger A. We used the than the lattice constant of the conventional cubic cell of diamond, a0 =3.54 ˚ Γ-point sampling in the Brillouin-zone which corresponds to sampling ﬁner than a 6 × 6 × 6 grid of the primitive lattice; this provides a well converged charge density. It is also advantageous to restrict the calculations to the Γ-point in order to keep the degeneracy of the e defect states which may split in a general k-point sampling of the Brillouin-zone. We checked that the geometry was practically identical (to within 0.01 ˚ A) going from a 216atom fcc supercell to the 512-atom simple cubic supercell. We will show that the calculated spin density, for instance, decays at much shorter distance than the lattice constant of the 8.

(10) supercell. Thus, the 512-atom supercell is adequate to represent the isolated NV defect in a realistic manner. We calculated the hyperﬁne tensor of the defect with the optimized geometry obtained by the VASP code. In the calculation of the hyperﬁne tensor the relativistic eﬀects are taken into account.45 The hyperﬁne tensor of nucleus I consists of the Fermi-contact term (ﬁrst parenthesis in the following equation) and the dipole-dipole term (second parenthesis): Z h 8π 3x x 1 δij i i j (I) d3 r ns (r)γI γeh ¯2 Aij = (4) δ(r) + − 2S 3 r5 r3 where ns (r) is the spin density of the spin state S, γI is the nuclear Bohr-magneton of nucleus I and γe is the electron Bohr-magneton. The Fermi-contact term is proportional to the spin density localized at the place of the nucleus which is dominant compared to the dipole-dipole term. The ratio of the Fermi-contact and dipole-dipole terms characterizes the shape of the spin density. The contribution of s-like wave functions to the charge density has a large eﬀect on the Fermi-contact term but negligible eﬀect on the dipole-dipole term, since the s-like wave function has a maximum at the positions of the nuclei and it is an even function. In contrast to this, the contribution of p-like wave functions to the charge density has a negligible eﬀect on the Fermi-contact term but a large eﬀect on the dipole-dipole term, since the p-like wave function has a node at the place of nuclei and it is an odd function. Typically, the contribution of the dipole-dipole term is signiﬁcant for the spin density built from welllocalized dangling bonds, that is, the sp3 hybrid orbitals (see Table II). We note that the pseudopotential methodology produces artiﬁcially smooth wave functions close to the nuclei, therefore only the all-electron PAW methodology can provide reliable hyperﬁne tensors. In the PAW methodology the calculation of the hyperﬁne tensor is somewhat more subtle than Eq. (4) shows and the dipole-dipole term is not fully calculated (see the appropriate note in Ref.45) which causes about 0.3 MHz inaccuracy in the calculated dipole-dipole term in our case. This error could be important to take into account for hyperﬁne tensors with small matrix elements (<3 MHz). The total spin density, ns (r), can be deﬁned as ns (r) = nup (r) − ndown (r) where nup (r) and ndown (r) are the spin densities built from spin-up and spin-down electrons, respectively. Taking the MS =1 state of the 3 A2 state, as shown in Fig. 2, we expect that 9.

(11) ns (r) will be positive. We will show that this is not true for the entire space around the defect.. IV. A.. ATOMIC AND ELECTRONIC STRUCTURE OF THE NV DEFECT Geometry and electronic levels. We begin with a discussion of the geometry optimization of the negatively charged NV center obtained from the SIESTA calculations using spin-polarization and no symmetry restrictions. The defect automatically ﬁnds t the S=1 state and maintains the C3v symmetry of the original, unrelaxed structure. The calculated one-electron defect levels are shown in Fig. 2. The ﬁrst neighbor C and N atoms clearly relaxed outward from the vacancy. The calculated distances from the vacant site are 1.63 and 1.69 ˚ A for the C atoms and the N atom, respectively, that is, the N atom relaxes more than the C atoms. We note that the C-vacancy distances are the same within 0.0002 ˚ A without any symmetry constraints after geometry optimization. The N-C bond lengths are 1.46 ˚ A, while the bond lengths of C radicals are 1.50 ˚ A, which is not far from 1.44 and 1.45 ˚ A, respectively, obtained in an LDA molecular cluster calculation.34 The localized basis sets can have problems in the description of vacancy-like defects. Our VASP calculation, which employs a plane wave basis set, shows basically the same geometry after optimization: the calculated distances from the vacant site are 1.62 and 1.68 ˚ A for the C atoms and the N atom, respectively. Thus, we conclude that the double-ζ plus polarization basis provides results very close to those of the converged plane wave basis set. In an earlier work by by Luszczek et al.,22 a plane wave basis set with pseudopotentials was employed in a 64-atom cubic supercell using 2 × 2 × 2 Monkhorst-Pack Brillouin Zone. sampling46 to investigate the NV defect in diamond. In that work, only the nearest neighbor. atoms to the vacant site were allowed to relax without symmetry restrictions and a geometry close to C3v symmetry was obtined; the largest deviation in the C-vacancy distances was about 0.001 ˚ A. The calculated distances from the vacancy were 1.67 and 1.66 ˚ A for the C atoms and the N atom, respectively, which shows the opposite trend from what we ﬁnd both in the SIESTA and in the VASP calculations in the larger unit cell. Most probably the diﬀerence is due to the insuﬃcient relaxation condition restricted only to the ﬁrst neighbor. 10.

(12) atoms around the vacant site. We plot the wave functions of the defect states obtained by the LSDA calculations in Fig. 3. The group theory analysis based on the single-particle picture describes very well <111>. (111). a1(1) <111>. (111). a1(2) <111>. (111). ex <111>. (111). ey. FIG. 3: (Color online) Isosurfaces of the calculated wavefunctions of the a1 (1), a1 (2), ex , ey defect states, shown in side (left) and top (right) views relative to the <111> axis. Blue (red) isosurfaces correspond to negative (positive) values of the wavefunction. The small pink circle represents the position of the vacant site, while the grey and cyan balls show the C and N atoms, respectively. We show the atoms up to the second neighbor from the vacant site.. the defect states. Naturally, the defect states are not strictly localized on the ﬁrst neighbor atoms of the vacancy but the largest portion of the wave functions can be indeed found 11.

(13) there. The SIESTA calculation gives α ≈ 0.7 for the parameter that appears in Eq. (1). This means that the N orbital is mostly localized on the a1 (2) : φ2 defect level and has no amplitude on the e levels. Therefore, the nitrogen atom is only very weakly spin-polarized in the 3 A2 state, while it is strongly spin-polarized in the 3 E state (when one electron is excited from the a1 (2) to level to the e level). This is clearly shown on Fig. 4. It is apparent, from this ﬁgure, that the N atom is only weakly polarized (small negative spin density) in the 3. A2 state while it is strongly polarized in the 3 E state comparable to the C ligands (large. positive spin density). The spin density is always highly localized on the three C atoms around the vacant site (orange lobes in the ﬁgure). <111>. 3. 3E. A2. −0.010 −0.005 +0.014 +0.070 +0.200. FIG. 4: (Color online) Calculated spin density isosurfaces in the MS =1 state for the 3 A2 (left) and the 3 E state (right). The vacant site is depicted by a small pink sphere at the center of each plot.. We also checked the situation when we optimized the geometry with the condition S=0. We already showed that the |σ2 σ¯2 σ3 σ¯3 i state is not an eigenstate with C3v symmetry. In addition, this state is a Jahn-Teller unstable system. Indeed, the defect reconstructs to C1h symmetry to remove the degenerate e level. However, this conﬁguration is about 0.3 eV higher in energy than the 3 A2 state with C3v symmetry.. 12.

(14) B.. Energy sequence of multiplets. From the structural analysis, we conclude that the dangling bonds around the vacancy do not form long bonds which could be the driving force of the reconstruction. Instead, the atoms relax outward from the vacancy and retain the strongly localized dangling bonds pointing to the vacant site which maintains the C3v symmetry. Since the degenerate e defect level is only partially occupied, this is a typical situation where conﬁgurational interaction plays a crucial role. As shown above, most of the singlet eigenstates can be described only by multi-determinantal wavefunctions in C3v symmetry. The optical transition takes place between the triplet states. We already showed the results on the 3 A2 state. In the VASP calculation it is possible to set the occupation of one-electron states. The 3 E state can be achieved by setting zero occupation for the spin-down φ2 level and full occupation of φ3 spin-up and spin-down levels. The energy of the 3 E state can be calculated in the ﬁxed geometry of the 3 A2 state which yields the vertical ionization energy. Upon the excitation of the electron the nuclei can relax to ﬁnd the minimum energy in the new conﬁguration space. This relaxation can take place with the help of phonons around the defect. The ZPL transition corresponds to that energy where phonons do not participate, between the energy minima of the two conﬁgurations as shown in Fig. 5.. FIG. 5: Energetics of photoluminescence absorption: VI is the vertical ionization energy, ZPL is the zero-phonon line transition, E is the total energy and Q the conﬁguration coordinate.. The calculated vertical ionization energy is 1.91 eV within LSDA. We found that the NV defect signiﬁcantly relaxes due to this internal ionization. The C-vacancy distance is 1.67 ˚ A while the N-vacancy distance is 1.61 ˚ A in the 3 E state. This shows the opposite trend than 13.

(15) what was found in the 3 A2 state. This may be understood as follows: the N atom is strongly spin-polarized in the 3 E state compared to 3 A2 state, while the C ligands will be somewhat less spin-polarized which induces diﬀerent charge transfer between the atoms in the 3 E state, and leads to a diﬀerent geometry. The calculated relaxation energy (the Fracnck-Condon shift) is 0.2 eV. From this, we ﬁnd a ZPL energy of 1.71 eV which can be tentatively compared to the experimental value of 1.945 eV.24,25 We note that a similar value (1.77 eV) was found by the LSDA molecular cluster calculation.34 The LSDA excitation energy and the experimental transition energy are remarkably close to each other. This shows that the self-interaction error of LSDA for these defect levels does not diﬀer too much, which is not unexpected since both of the defect states are basically valence band derived (from sp3 -like hybrid orbitals). Nevertheless, the calculated Franck-Condon shift, which is the relaxation energy deﬁned as the energy diﬀerence between the vertical ionization energy and the ZPL energy, should be even more accurate than the calculated internal ionization energy. Indeed, the PL spectrum shows a broad phonon spectrum even at low temperature, and the intensity of the ZPL line is relatively small compared to the phonon side bands which indicates a large Franck-Condon shift. In addition to the triplet states it is worthwhile to calculate the energies of the singlet states because they play a signiﬁcant role in the emission process but these states have not yet been measured directly in experiments (see Ref.23 and references therein). LSDA is not a suitable methodology to calculate these energies accurately. Beside the self-interaction error (which is relatively small for these defect levels as discussed above), LSDA gives the charge density of the interacting electrons, which is expressed in terms of the non-interacting Kohn-Sham particles. In the Hartree-Fock language the total wave function, which is not directly used in DFT-LSDA, is expressed by a single Slater-determinant. Thus, the usual DFT-LSDA calculation cannot represent most of the singlet eigenstates of the NV center. This can be corrected by using a perturbation theory within DFT-LSDA as explained by Lannoo et al..47 Instead, we adopt here a more approximate method48 which was already applied for some states of this defect in Ref.34. Our goal is to give approximate energies of the singlet eigenstates in order to predict their sequence, and we do not attempt to provide energies directly comparable to the experiments. One of the 1 A1 states can be described by a single Slater-determinant (when the a1 (2) level is totally empty and the e level is fully occupied). This state can be calculated with geometry 14.

(16) optimization by LSDA as explained for the 3 E state. We therefore concentrate on the remaining 1 A1 and two 1 E states. While the |σ2 σ¯2 σ3 σ¯3 i, |σ2 σ¯2 σ3 σ¯4 i, and |σ2 σ3 σ¯3 σ¯4 i single Slater-determinants are not eigenstates, they can be expressed as the linear combination of diﬀerent eigenstates shown in Eqs. (2a), (2b) and (3). von Barth48 has shown that the LSDA total energy (E) of the mixed state can be expressed as the appropriate sum of the energy of the eigenstates, which yields the following equations: 1 E[|σ2 σ¯2 σ3 σ¯4 i] = (E[1 E] + E[3 A2 ]) 2 1 E[|σ2 σ¯2 σ3 σ¯3 i] = (E[1 E] + E[1 A1 ]) 2 1 E[|σ¯2 σ3 σ4 σ¯4 i] = (E[3 E] + E[1 E]) 2. (5a) (5b) (5c). In Eqs. (5a) and (5c) we assume that the energy of the triplet states with MS = 0 and MS = 1 is the same. This is a very good approximation since, for instance, the experimentally measured splitting is about 2.88 GHz (few µeV) for the ground state due to spin-spin interaction,16 while the spin-orbit splitting for the 3 E state is expected to be within few meV, which is far beyond the accuracy of LSDA calculations. The energy of the mixed states on the left hand side of Eqs. (5a)-(5c) can be calculated directly by LSDA. Since E[3 A2 ] is. known, E[1 E] can be determined from Eq. (5a). Similarly, E[1 E] can be determined from. Eq. (5c). By combining Eqs. (5a) and (5b) we arrive at: E[1 A1 ] = 2(E[|σ2 σ¯2 σ3 σ¯3 i] − E[|σ2 σ¯2 σ3 σ¯4 i]) + E[3 A2 ]). (6). Thus, the 1 A1 state can be also determined. von Barth48 applied this approach successfully to calculate the energy of atoms in diﬀerent states. Formally, this method can also be applied to the NV defect in diamond, but attention must be paid to relaxation eﬀects. Generally, if the electron state changes then it may imply also relaxation of the ionic positions, as was the case for the 3 E state discussed earlier. Relaxation eﬀects cannot be taken into account with this methodology, since only the energy of the mixed states can be calculated directly by LSDA, and the relaxation of the mixed state is meaningless. In other words, the geometry must be ﬁxed in these calculations. The occupation of the e state varies in the case of the 1 A1 and 1 E states of the a21 (2)e2 conﬁguration. We assume that the geometry would involve negligible change from the geometry of the 3 A2 state which belongs also to the a21 (2)e2 conﬁguration. Therefore, 15.

(17) we ﬁx the geometry obtained in the 3 A2 state in the process of calculating the 1 A1 and 1 E states of the a21 (2)e2 conﬁguration. Using the same argument we ﬁx the geometry obtained for the 3 E state in the calculation of the 1 E state of the a11 (2)e3 conﬁguration. With these, we ﬁnd the following energy sequence of the multiplets: ≈0.0 eV. ≈0.9 eV. ≈0.8 eV. ≈0.5 eV. ≈1.3 eV. E[3 A2 ] −−−−−→ E[1 A1 ] −−−−−→ E[1 E] −−−−−→ E[3 E] −−−−−→ E[1 E] −−−−−→ E[1 A1 ], that is, the deeper 1 A1 state is close in energy to the 3 A2 state, and the deeper 1 E state is below 3 E state. The energy diﬀerences between the triplet states were already discussed. We focus next on the singlet states. Within our approximate methodology the 3 A2 and 1 A1 states are almost degenerate. Close inspection of Eq. (6) reveals that the energy sequence of the 3 A2 and 1 A1 states depends on the energy diﬀerence of two singlet states: (E[|σ2 σ¯2 σ3 σ¯3 i] − E[|σ2 σ¯2 σ3 σ¯4 i]). We obtain almost zero for this energy diﬀerence. However, the LSDA self-interaction error may be larger for the |σ2 σ¯2 σ3 σ¯3 i state (where the exchange energy of σ3 appears) than for the |σ2 σ¯2 σ3 σ¯4 i state (where the electrons occupy spatially. orthogonal orbitals). This may raise the energy of the E[1 A1 ] state. Nevertheless, this can be partially compensated by the relaxation eﬀect of the 1 A1 state which we are neglecting. by necessity as explained before. An additional issue is the possible mixing with the higher 1. A1 state. We argue that the two 1 A1 states are not likely to mix because they are very far. from each other in energy. We conclude from the above analysis that the 1 A1 state is indeed close in energy to the 3. A2 state. This may imply a very complicated ﬁne structure of the states. Taking the spin-. spin interaction into account the 3 A2 state splits to A1 (MS = 0) and E(MS = ±1) states,. while 1 A1 becomes A1 (MS = 0) (the spin state is not a good quantum number anymore,. just its projection). If the two A1 (MS = 0) states are close in energy then they may mix with each other. It is also important to notice that the energy of the deeper 1 E state falls between the energies of the triplet states. The relaxation eﬀect may lower the energy of this state. In addition the two 1 E states are not far from each other in energy, so the oﬀ-diagonal elements in the hamiltonian may not be neglected. The mixing of the two 1 E states would further lower the energy of the deeper 1 E state and would raise the energy of the higher 1 E state. The ﬁnal conclusion is that there are two singlet states between the triplet states, and the 1 A1 state is much closer in energy to the ground state than the 1 E state. The energies of the other two singlet states are certainly above that of the 3 E state. 16.

(18) The deeper singlet 1 A1 and 1 E states can play an important role in the emission process of the NV center. Experiments indicate that there should be a possibly long-living singlet state between the triplet states (see Ref.23 and references therein). Usually, the singlet 1 A1 is considered in this process. However, our calculations indicate that there are two singlet states between the triplet states. Goss et al.34 reported the sequence of 3 A2 , 1 E, 1 A1 , and 3 E states which is surprising in light of the previous discussion, as these states were obtained by LSDA molecular cluster calculations. Manson et al.23 recently showed that if the 1 E state is above the 1 A1 state, the known properties of the emission can be consistently explained as with the original singlet 1 A1 model, with the only diﬀerence being that the 1 E and 1 A1 states both contribute to the spin polarization process during the optical cycling and that the eﬀect will be more eﬃcient. Having the 1 A1 state higher in energy than the 1 E state would result in no change in spin orientation during optical cycling which is in contradiction with experiment.23 From this point of view our results obtained from approximate calculations are consistent with the PL experiments.. V.. HYPERFINE CONSTANTS. As mentioned in the Introduction, the NV center in diamond is a promising candidate to realize qubit solid state devices operating at room temperature (Ref.14 and references therein). The qubit is the non-zero (S=1) electron spin ground state which can interact with the neighbor 13 C isotopes possessing I=1/2 nuclear spin via hyperﬁne interaction. The natural abundance of the. 13. C isotope is about 1.1%, so we can assume the same abundance. in the diamond lattice. In conventional EPR measurements, the EPR absorption signal is detected on the ensemble of the defects in the diamond sample. The sample should be thick enough for absorption measurements and the concentration of the defects should be suﬃciently high. Finally, a large number of defects is measured at the same time by EPR, so statistics can be applied to analyze the data. If the spin density is strongly localized on three symmetrically equivalent C ligands (see Fig. 4) then the probability of ﬁnding one 13 C atom among them is given by the binomial distribution and is about 3.2%. Finding two or three of them has negligible probability. Due to the I=1/2 nuclear spin, the hyperﬁne interaction splits to two lines with Iz = 1/2 and Iz = −1/2 and therefore the intensity ratio between the main hyperﬁne line (involving no hyperﬁne interaction with 17. 13. C atoms) and.

(19) the hyperﬁne line associated with the C ligands will be roughly 1.5%. This makes the EPR measurement on. 13. C hyperﬁne interaction a challenging task, since the signal to noise ratio. should be very good and the intensity of the EPR signal should be strong enough and stable to identify the satellite hyperﬁne lines due to. 13. C isotopes.. The 13 C hyperﬁne interaction has been detected in EPR from two sets of three symmetrically equivalent C atoms by Loubser and van Wyk.16,49 The larger hyperﬁne constants were associated with the C-ligands of the NV center. In addition, the hyperﬁne interaction of the. 14. N isotope was found in NV center by EPR and ENDOR measurements.16,17 To our. knowledge, hyperﬁne interaction with other. 13. C isotopes has not been measured directly by. EPR. We can estimate the localization of the charge density on the C and N atoms that are immediate neighbors of the vacant site, from the linear combination of the atomic orbitals as they appear in the wavefunctions. He et al.17 estimated that 72% and 0.2% of the charge density is localized on the three C ligands and the N atom, which leaves approximately 28% of the charge density to be spread in the lattice. Wrachtrup et al.3 speculated that the spin density decays exponentially as a function of the distance from the vacant site. Since the hyperﬁne constants are roughly proportional to the spin density, as Eq. ((4)) indicates, these authors proposed that 9 or more carbon nuclei should have a hyperﬁne value of 70 MHz in the second neighborhood while the more distant carbon atoms should have a hyperﬁne constant smaller than 10 MHz. This proposal is not entirely consistent with the known EPR data, since isotropic hyperﬁne splitting of 5.4 G(≈15 MHz) was measured from three 13. C isotopes49 whereas a value of 70 MHz hyperﬁne splitting should be measurable by EPR. because it would not be obscured by the main EPR line. In their theoretical treatment of the NV center, Luszczek et al.22 claimed that they can support the proposal of Wrachtrup et al.3 based on their ab initio results. They optimized the geometry without symmetry constraints only for the ﬁrst neighbor atoms of the vacancy in a 64-atom supercell. The adequacy of this restriction was already discussed above; with this restriction, while the C3v symmetry is almost retained, the calculated Fermi-contact hyperﬁne interactions for the three C ligands deviate from each other more than 10% (see Table 2 in Ref.22). This suggests that the spin density was not adequately converged in that calculation since the small deviation in the geometry from the C3v symmetry could not imply such a large discrepancy in the calculated hyperﬁne ﬁeld. These authors also calculated the Fermi-contact hyperﬁne interaction for the C atoms situated about 2.5 ˚ A away from the 18.

(20) vacant site. The reported numbers were about an order of magnitude smaller than for the C ligands, which led to their conclusion that the spin density and the corresponding hyperﬁne constants should decay fast for other C-atoms farther from the vacant site. In addition to the problem of the inconsistent values of the hyperﬁne interaction for the three C-ligands, several other issues related to the results of Ref.22 must be mentioned: (i) These authors reported actually the hyperﬁne field and not the hyperﬁne constant. However, the conversion from the hyperﬁne ﬁeld, which is the magnetization density on the atom and it is a number directly obtained from the computation, to the hyperﬁne constant is not unique; therefore, it is very diﬃcult to compare the calculated values to the experimental data. (ii) Only the Fermi-contact term was calculated while the dipole-dipole term can be also signiﬁcant; this is known to be the case for the C ligands from experimental measurements.16,49 (iii) The hyperﬁne interaction with distant C atoms could be very important for qubit applications based on this defect, so the hyperﬁne tensor must be calculated at larger distances from the vacancy. Based on these arguments, we believe that the nature of the spin density and the corresponding hyperﬁne interaction with the. 13. C isotopes has not yet been explored in detail. despite of its high importance. Toward establishing the nature of this interaction, we show ﬁrst the calculated spin density in our 512-atom supercell in Fig. 6. As expected, the spin density is highly localized around the three C-ligands nearest to the vacant site (orange lobes in the ﬁgure), within a radius of 1 × a0 from this site. The spin density practically vanishes at distances > 2 × a0 from the vacant site. Below the three C atoms (see Fig. 6) there is the N atom with a small negative spin density. Some C atoms farther from the vacant site also have negative spin density. The spin density extends mostly on a plane perpendicular to the (111) direction and no measurable spin density can be found below the N atom. On the N atom, the spin density is negative. It was shown earlier that the spin density comes mostly from the spin-polarized e level localized on the C dangling bonds, and due to symmetry reasons, orbitals related to the N do not appear in the e level. The tiny negative charge density on the N atom can be explained by the polarization of its core states: since the nuclear Bohr-magneton of the N atom is positive, the Fermi-contact term will be negative (see Table II). Overall, the spin density is spread on a plane perpendicular to the (111) direction. There are some C atoms 19.

(21) <111>. o. 14.2 A = 4 x a0. (a). −0.010 −0.005 +0.014 +0.070 +0.200. (111). (b). (c). FIG. 6: (Color online) (a) The 512-atom cubic supercell with all C atoms shown (atoms within a 64-atom supercell are shown in red). The suprercell size in ˚ A and in units of the conventional cubic cell lattice constant, a0 , is indicated on the side of the cube. (b) Perspective view of the calculated spin density isosurfaces in the MS =1 state. Only atoms up to the second nearest neighbor of the vacant site are shown. (c) View along the (111) direction indicating the C3v symmetry of the spin density, which is given in colored contours. The black lines denote the size of the 512-atom supercell, while the red dotted ones show the boundaries of the 64-atom supercell.. which have signiﬁcant negative spin density which results in negative Fermi-contact term. No measurable hyperﬁne interaction (spin density) can be found for the C atoms below the N atom. Loubser and van Wyk49 speculated that the 15 MHz. 13. C isotropic hyperﬁne. splitting comes from the three C atoms bonded to the N atom. Our calculation negates this possibility. Table II shows that there is a local maximum of the spin density at Rvac ≈3.9 and 5.0 ˚ A,. where Rvac is the distance from the vacant site. At Rvac >6.3 ˚ A the calculated hyperﬁne. constants are below 1 MHz which means that the spin density vanishes at Rvac ≈ 2×a0 . Apparently, the 64-atom supercell is too small to capture these properties due to the artiﬁcial overlap of the spin density caused by the periodic boundary conditions. We also ﬁnd that the charge density does not decay monotonically like an exponential function, but behaves more like a wavepacket, that is, as f (x) = sin(x)/x (see Fig. 7). It is important to compare the calculated hyperﬁne values with the known experimental data in order to estimate the accuracy of our calculations. For that purpose, the hyperﬁne constant of the N atom is not the best choice because its value is very small and it is 20.

(22) TABLE II: The calculated principal values of the hyperﬁne tensor (columns 3 to 5) compared to the known experimental data (columns 6 to 8) in MHz. The average of the three principal values yields the Fermi-contact term. The diﬀerence between the principal values and the Fermicontact term gives the dipole-dipole term. Only atoms with a signal larger than 2 MHz are shown. The symmetrically equivalent number of C atoms is shown in the ﬁrst column and their distance in ˚ A from the vacant site in the second column. The experimental data on Refs.17,49. Experimental data on. 13 C. 14 N. is taken from. atoms were taken from Ref.49. EPR studies can directly. measure only the absolute value of the hyperﬁne constants, which is indicated by adding a ± sign to experimental values. The calculated hyperﬁne tensors can be used for comparison with spin-echo measurements (see text). Atom. Rvac. A11. A22. A33. Aexp 11. Aexp 22. Aexp 33. 14 N. 1.68. -1.7. -1.7. -1.7. ±2.1. ±2.1. ±2.3. 3C. 1.61. 109.5. 110.2. 185.4. ±123. ±123. ±205. 6C. 2.47. -4.8. -3.7. -1.5. 3C. 2.49. -7.4. -7.3. -5.8. 6C. 2.90. 2.8. 3.3. 4.6. 3C. 2.92. 1.4. 2.4. 2.9. 3C. 2.93. 3.4. 4.7. 4.9. 6C. 3.85. 13.5. 14.2. 19.4. 3C. 3.86. 12.8. 12.8. 18.0. ±15.0. ±15.0. ±15.0. 6C. 4.99. 2.6. 2.7. 3.8. 3C. 5.00. 1.5. 1.5. 2.2. caused by only indirect spin-polarization eﬀect. As mentioned above, there is an inherent inaccuracy in the calculated dipole-dipole term of about 0.3 MHz, therefore it is reasonable to consider only values of the hyperﬁne constants that are signiﬁcantly larger than this limit. Accordingly, we restrict the comparison to values that are higher than 2 MHz. By comparing the hyperﬁne constants of the C-ligands we estimate the inaccuracy for both the Fermi-contact term and the dipole-dipole term to be about 10%. This is usual for LSDA calculations.18,19,20,21 The calculated ratio between the Fermi-contact term and the dipole-. 21.

(23) 190 15. Aij (MHz). 140. 90. 5 −5 2.5. 4. 5.5. 7. A11 A33. 40. −10 1.5. 3. 4.5. Rvac (Α). 6. 7.5. o. FIG. 7: Variation of the principal values of the hyperﬁne tensor A11 and A33 as a function of the distance from the vacant site (Rvac ) for the set of 3 symmetrically equivalent C atoms (3C). In the inset we show changes farther from the vacant site on a ﬁner scale. The variation for the set of 6 symmetrically equivalent C atoms follows closely the one shown for 3C.. dipole term agrees remarkably well with experiment for the C-ligands. This shows that the shape of the spin density is very well described by LSDA. This ratio indicates that the p-functions dominate by about 90% in the dangling bonds, so those are more p-like orbitals than sp3 hybrids. The reason is most likely the outward relaxation of the C-atoms from the vacant site. The plotted wavefunctions indeed show a very strong p-contribution of the e levels in Fig. 3 while the spherical s-contribution is very small. The shape of the wave functions can be directly compared to the proposed wave functions in Eq. (1) from the group theory analysis of the defect diagram. An additional 15 MHz 13 C hyperﬁne splitting was measured by Loubser et al.49 using EPR but the measured spectrum of the NV center was not shown in detail, therefore we cannot comment on the accuracy of this measurement. Nevertheless, that work stated that the hyperﬁne splitting is isotropic, that is, the dipole-dipole term is negligible, and the relative intensity of the hyperﬁne satellite line and the main EPR line indicates the involvement of three symmetrically equivalent C atoms.49 The likely candidate for this signal is found at the third neighbors of the vacant site at Rvac =3.86 ˚ A. The spin density of these atoms is shown as yellow lobes above the small green lobes at the highest position on the side view in Fig. 6. The calculated anisotropy of this hyperﬁne interaction is about 3-4 MHz. If the uncertainty in the measurement is in this range due to line broadening, then the signal could 22.

(24) be detected as nearly isotropic. However, our calculations reveal that six additional C atoms have similar hyperﬁne splitting at the third neighbor distance of Rvac =3.85 ˚ A, corresponding to the six yellow lobes laterally spread farthest from the vacant site, which is most obvious from the view along the (111) direction in Fig. 6. This means that the hyperﬁne splitting due to these six C atoms would have to be detected simultaneously with the other three ones. Since the diﬀerence in the hyperﬁne splitting of these two sets of atoms is small, the six-atom set could obscure the signal of the three-atom set showing an eﬀective relative intensity associated with six symmetrically equivalent C atoms. We suggest that this part of the spectrum should be re-investigated in detail experimentally. The hyperﬁne splitting of 7-8 MHz from the. 13. C atom may be also detectable by EPR while the other signals may. be too small and hence obscured by the main hyperﬁne lines. Recently, individual NV centers have been detected by spin-echo measurements.13,14 In particular, detailed results for six NV centers in diamond have been reported.13 The spin-echo measurements have detected the coherent state of the electron spin coupled with a proximal 13. C nucleus. The coupling is due to hyperﬁne interaction between the electron spin and. the nuclear spin of. 13. C isotopes. The resulting spin-echo signals show a rapidly oscillating. function enveloped by a more slowly oscillating function.13 These authors proposed a theory to explain this signal, and they concluded that the fast modulation frequency is due to the eﬀective magnetization density of the electron spin felt by the 13 C nucleus, which is the same as the hyperﬁne interaction. The modulation frequency can be well approximated as the norm of the hyperﬁne tensor projected to the symmetry axis, which leads to the following expression within our formulation of the problem: q (X) 2 (X) ω = [111] × Aij (X). where [111] is the appropriate projection vector and Aij (X). X. Since we calculate the full Aij. (7) is the hyperﬁne tensor of nucleus. tensor (see Eq. (4)), the calculation of the modulation. frequency is straightforward. Modulation frequencies have been reported for four single NV defects (see Fig. 4B in Ref.13). A single modulation frequency was measured for each NV center at ≈2 MHz, ≈4 MHz, ≈9 MHz, and ≈14 MHz, respectively, so these particular NV centers had hyperﬁne interaction with one. 13. C isotope in the lattice.13 It would be useful. to compare the hyperﬁne interaction measured by EPR and spin-echo techniques which can be an additional validation of the theory developed by Childress and co-workers.13 As was 23.

(25) explained earlier, conventional EPR tools have limitations in detecting. 13. C isotopes. A. 13. C. enriched sample would be useful to study this defect experimentally in more detail. The largest. 13. C hyperﬁne splitting corresponds to a modulation frequency that is too. large to be detected by spin-echo measurements. However, an isotropic. 13. C hyperﬁne split-. ting of 15 MHz has also been reported.49 The isotropic signal means that the modulation frequency should be also about 15 MHz. This is very close to one of the measured modulation frequencies at ≈14 MHz.13 From the calculated hyperﬁne tensors in Table II, this signal must originate from a C-atom which is a third neighbor of the vacant site at Rvac =3.86 ˚ A.. The calculated modulation frequency is ≈16 MHz which is close to the measured one taking into account the limitations of our computational method. The 9 MHz spin-echo signal can originate only from the atoms at Rvac =2.49 ˚ A, and contributions from other neighbors can be safely excluded. In this way, the origin of the signal can be identiﬁed. The 4 MHz A taking A or at Rvac =2.93 ˚ spin-echo signal can originate either from atoms at Rvac =2.90 ˚ into account computational limitations. In the ﬁrst case, six symmetrically equivalent C atoms are involved, while in the second case a set of three symmetrically equivalent C atoms are involved. It is diﬃcult, if not impossible, to identify the origin of the 1 MHz spin-echo signal, which is beyond the accuracy of our calculations. Nevertheless, the calculations indicate that this signal could arise from at least 12 C atoms. Most of them are far from the vacant site but some are closer than the atoms that give rise to the ≈14 MHz signal, as is evident from Figure 7. The number of symmetrically equivalent atoms is also speciﬁc to the individual hyperﬁne constant, and therefore to the modulation frequency. Because of the C3v symmetry, sets of three or sets of six C atoms are equivalent with each other. The relative occurrence of the modulation frequencies measured by spin-echo experiments helps in identifying the equivalent atoms around the vacancy. Four samples represent a rather limited set of values for statistical analysis, so the relative occurrence of. 13. C isotopes picked up by these measure-. ments cannot be used for such analysis. A much larger number of NV samples is needed in the spin-echo measurements in order to use the relative occurrence of the 13 C isotope signals for the identiﬁcation of individual atoms in the diamond lattice.. 24.

(26) VI.. SUMMARY AND CONCLUSIONS. In this work we investigated the negatively charged nitrogen-vacancy center in diamond in detail by ab initio supercell calculations using density functional theory methods. We showed that the energy sequence of multiplet states is 3 A2 , 1 A1 , 1 E, 3 E, 1 E, and 1 A1 . This means that the singlet 1 E state enhances the spin polarization process during the optical cycling of the defect. The center has non-zero spin ground state. The full hyperﬁne tensor for a large number of atoms around the defect was calculated for the ﬁrst time. The calculated hyperﬁne constants of the C ligands agree well with the experimental values detected by electron paramagnetic resonance tools. However, there is a controversy about the number of symmetrically equivalent carbon atoms of the second highest hyperﬁne interactions when these are compared to experiment. We propose that that part of the electron paramagnetic resonance spectrum should be re-investigated in detail in order to clarify this issue. Our calculations reveal that the spin density of the ground state is spread in the lattice, mostly on a plane perpendicular to the (111) direction deﬁned by the positions of the N atom and the vacant site, and that it does not decay monotonically from the vacant site. As a consequence, only a certain number of 13 C isotopes can interact with the electron spin, which can be used as qubits for quantum computing. Using the limited number of measurements that have been recently published for single nitrogen-vacancy centers detected by spin-echo measurements, we were able to identify some individual atoms around the defect. Our results contribute to the understanding of the spin-echo signals of the defect, which is a crucial step towards realization of the qubit concept in this system. Additional spin-echo measurements in NV samples will help identify other individual. 13. C atoms around the defect.. Acknowledgments. We are thankful to Liang Jiang, Jeronimo Maze and Mikhail Lukin for encouraging discussions. AG acknowledges support from E¨otv¨os Fellowship of Hungary. MF acknowledges support by Harvard’s Nanoscale Science and Engineering Center, funded by the National. 25.

(27) Science Foundation, Award Number PHY-0117795.. 1. A. Gruber, A. Drabenstedt, C. Tietz, L. Fleury, J. Wrachtrup, and C. Borczyskowski, Science 276, 2012 (1997).. 2. A. Drabenstedt, L. Fleury, C. Tietz, F. Jelezko, S. Kilin, A. Nizovtzev, and J. Wrachtrup, Physical Review B 60, 11503 (1999).. 3. J. Wrachtrup, S. Y. Kilin, and A. P. Nizotsev, Opt. Sepctrosc. 91, 429 (2001).. 4. F. Jelezko, I. Popa, A. Gruber, C. Tietz, J. Wrachtrup, A. Nizovtsev, and S. Kilin, Appl. Phys. Lett. 81, 2160 (2002).. 5. F. Jelezko, T. Gaebel, I. Popa, A. Gruber, and J. Wrachtrup, Phys. Rev. Lett. 92, 076401 (2004).. 6. F. Jelezko, T. Gaebel, I. Popa, M. Dunham, A. Gruber, and J. Wrachtrup, Phys. Rev. Lett. 93, 130501 (2004).. 7. R. J. Epstein, F. Mendoza, Y. K. Kato, and D. D. Awschalom, Nat. Phys. 1, 94 (2005).. 8. R. Hanson, F. M. Mendosa, R. J. Epstein, and D. D. Awschalom, Phys. Rev. Lett. 97, 087601 (2006).. 9 10. R. Brouri, A. Beveratos, J.-P. Poizat, and P. Gragier, Opt. Lett. 25, 1294 (2000). A. Beveratos, R. Brouri, T. Gacoin, J.-P. Poizat, and P. Grangier, Phys. Rev. A 64, 061802(R) (2002).. 11. L. Childress, J. M. Taylor, A. S. Sørensen, and M. D. Lukin, Phys. Rev. Lett. 96, 070504 (2006).. 12. L. Jiang, J. M. Taylor, A. Sørensen, and M. D. Lukin, quant-ph/0703029 (2007).. 13. L. Childress, M. V. Gurudev Dutt, J. M. Taylor, A. S. Zibrov, F. Jelezko, J. Wrachtrup, P. R. Hemmer, and M. D. Lukin, Science 314, 281 (2006).. 14. M. V. Gurudev Dutt, L. Childress, L. Jiang, E. Togan, J. Maze, F. Jelezko, A. S. Zibrov, P. R. Hemmer, and M. D. Lukin, Science 316, 312 (2007).. 15. Cappellaro, unpublished.. 16. J. H. N. Loubser and J. P. van Wyk, in Diamond Research (London) (Industrial Diamond information Bureau, London, 1977), pp. 11–15.. 17. X.-F. He, N. B. Manson, and P. T. H. Fisk, Phys. Rev. B 47, 8816 (1993).. 18. T. Umeda, Y. Ishitsuka, J. Isoya, N. T. Son, E. Janz´en, N. Morishita, T. Ohshima, H. Itoh,. 26.

(28) and A. Gali, Phys. Rev. B 71, 193202 (2005). 19. T. Umeda, N. T. Son, J. Isoya, E. Janz´en, T. Ohshima, N. Morishita, H. Itoh, A. Gali, and M. Bockstedte, Phys. Rev. Lett. 96, 145501 (2006).. 20. N. T. Son, P. Carlsson, J. ul Hassan, E. Janz´en, T. Umeda, J. Isoya, A. Gali, M. Bockstedte, N. Morishita, T. Ohshima, and H. Itoh, Phys. Rev. Lett. 96, 055501 (2006).. 21. T. Umeda, J. Ishoya, T. Ohshima, N. Morishita, H. Itoh, and A. Gali, Phys. Rev. B 75, 245202 (2007).. 22. M. Luszczek, R. Lakowski, and P. Horodecki, Physica B 348, 292 (2004).. 23. N. B. Manson, J. P. Harrison, and M. J. Sellars, Physical Review B 74, 104303 (2006).. 24. L. du Preez, PhD. dissertation, University of Witwatersrand, 1965.. 25. G. Davies and M. F. Hamer, Proc. R. Soc. London Ser. A 348, 285 (1976).. 26. A. T. Collins, J. Phys. C 16, 2177 (1983).. 27. R. Hanson, O. Gywat, and D. D. Awschalom, Phys. Rev. B 74, 161203 (2006).. 28. D. A. Redman, S. Brown, R. H. Sands, and S. C. Rand, Phys. Rev. Lett. 67, 3420 (1991).. 29. N. R. S. Reddy, N. B. Manson, and C. Wei, J. Lumin. 38, 46 (1987).. 30. E. van Oort, N. B. Manson, and M. Glasbeek, J. Phys. C 21, 4385 (1988).. 31. N. B. Manson, P. T. H. Fisk, and X.-F. He, Appl. Magn. Reson. 3, 999 (1992).. 32. J. P. Goss, R. Jones, P. R. Briddon, G. Davies, A. T. Collins, A. Mainwood, J. A. van Wyk, J. M. Baker, M. E. Newton, A. M. Stoneham, and S. C. Lawson, Phys. Rev. B 56, 16031 (1997).. 33. A. Lenef and S. C. Rand, Phys. Rev. B 56, 16033 (1997).. 34. ¨ J. P. Goss, R. Jones, S. J. Breuer, P. R. Briddon, and S. Oberg, Phys. Rev. Lett. 77, 3041 (1996).. 35. A. Lenef and S. C. Rand, Phys. Rev. B 53, 13441 (1996).. 36. D. M. Ceperley and B. J. Alder, Phys. Rev. Lett. 45, 566 (1980).. 37. J. P. Perdew and A. Zunger, Phys. Rev. B 23, 5048 (1981).. 38. G. Kresse and J. Hafner, Phys. Rev. B 49, 14251 (1994).. 39. G. Kresse and J. Furthm¨ uller, Phys. Rev. B 54, 11169 (1996).. 40. D. Sanch´ez-Portal, P. Ordej´ on, E. Artacho, and J. M. Soler, Int. J. Quantum Chem. 65, 543 (1997).. 41. N. Troullier and J. L. Martins, Phys. Rev. B 43, 1993 (1991).. 42. P. E. Bl¨ochl, Phys. Rev. B 50, 17953 (1994).. 27.

(29) 43. G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 (1999).. 44. P. E. Bl¨ochl, C. J. F¨orst, and J. Schimpl, Bull. Mater. Sci. 26, s33 (2001).. 45. P. E. Bl¨ochl, Phys. Rev. B 62, 6158 (2000).. 46. H. J. Monkhorst and J. K. Pack, Phys. Rev. B 13, 5188 (1976).. 47. M. Lannoo, G. A. Baraﬀ, and M. Schl¨ uter, Phys. Rev. B 24, 943 (1981).. 48. U. von Barth, Phys. Rev. A 20, 1693 (1979).. 49. J. H. N. Loubser and J. A. van Wyk, Rep. Prog. Phys. 41, 1201 (1978).. 28.

(30)